- Nano Express
- Open Access
Controlled Synthesis of BaYF5:Er3+, Yb3+ with Different Morphology for the Enhancement of Upconversion Luminescence
Nanoscale Research Letters volume 12, Article number: 633 (2017)
In this work, Er3+/Yb3+-codoped BaYF5 with different sizes and shapes have been synthesized by a simple solvothermal method. By changing the fluoride source, pH value, solvent, surfactants, Yb3+ concentration, temperature, and reaction time, the optimum synthetic conditions of BaYF5:Er3+, Yb3+ were found to improve the upconversion luminescent properties. It is found that the emission intensity of green and red light is enhanced for several times by the way of using NaBF4 as a fluoride source with the comparison of NH4F and NaF. Moreover, the effects of different surfactants are not the same. Adding 5% polyetherimide (PEI) as surfactant can also improve the upconversion emission. On the contrary, when sodium citrate (CIT) as another surfactant was used to add, the sizes of the nanocrystals were gradually increased and the luminous properties also declined.
In recent year, upconversion nanophosphors (UCNPs) have attracted increasing attention due to their use in many fields such as solid state laser devices, fluorescent probe imaging, bioapplication, stereoscopic three-dimensional display, infrared quantum counter, temperature sensor, and anti-fake [1,2,3,4,5,6,7,8,9,10,11]. UCNPs are usually composed of matrix material, activator, and sensitizer . Because of its low phonon energy and excellent chemical stability, fluorides are often used as matrix materials for the preparation of UCNPs. NaYF4  nanoparticles with good upconversion emission have a hexagonal phase structure, while the cubic phase results in poor upconversion emission. Recently, some of the UC materials based on BREF5 (B = Mg, Ba, Ca, Sr) have also been studied and these newly developed crystals were found to be suitable for UC applications [14, 15]. Er3+-doped BaYF5 extremely exhibits the strong UC luminescence ability. The luminescence intensity of Er3+-doped BaYF5 is eight times that of Er3+-doped LaF3 . When Er3+ is used as activator, Yb3+ is a representative UC luminescence sensitizer due to their efficient energy transfer [17,18,19,20,21]. Moreover, the charge sizes of Er3+ and Y3+ match, and their radii are similar (Er3+ radius is 0.1 nm, Y3+ radius is 0.101 nm) . Therefore, BaYF5 is deemed to be an appropriate host for Er3+ ions.
The main factors affecting the luminescence properties are particle size, morphology, structure, and others [23, 24]. In order to obtain UC luminescent materials with high efficiency, the controlled synthesis of the spherical particles with suitable size is beneficial to achieve high accumulation of density and scatter light. In this work, samples of Yb3+/Er3+-codoped BaYF5 are fabricated by a solvothermal method. Under the different reaction conditions, the samples with different morphologies and properties were synthesized. NaBF4 as fluoride source has a higher UC luminous intensity relative to NH4F and NaF. Perhaps it can slowly release F−; thus, it is more conducive to make crystal growth and promote UC luminescence. Furthermore, the influence of solvent, surfactants, Yb3+ concentration, pH of initial solution, temperature, and reaction time was also reported. Between UC luminous efficiency and various reaction conditions, the regularity and mechanism have been investigated.
All the chemicals are analytical grade, such as Ba(OH)2·xH2O, Y(NO3)3·6H2O, Yb2O3, (CH3CO2)3Er, NaBF4, NH4F, NaF, oleic acid, and HNO3, and absolute ethanol was used. Deionized water was used throughout. All chemical materials were used as received without further purification.
Preparation of Synthetic BaYF5:Er3+, Yb3+
Yb2O3 was dissolved in dilute HNO3 by heating the solution in order to gain the Yb(NO3)3 solution. In a typical synthetic route, Ba(OH)2·xH2O, Y(NO3)3·6H2O, (CH3CO2)3Er, and NaBF4 were separately dissolved in deionized water. According to the ratio of BaY1-x-yF5:xEr3+, yYb3+, the solution of Ba(OH)2·xH2O, Y(NO3)3·6H2O, (CH3CO2)3Er, Yb(NO3)3, and NaBF4 were put into a Teflon cup. Oleic acid and ethanol were added into the mixture for corresponding to a certain proportion. The pH value of the mixed solution was adjusted to 9 by using NH3·H2O. After magnetic stirring for 30 min, the Teflon cup was held into stainless steel sealing autoclave and heated to 200 °C for 16 h. When the autoclave was naturally cooled to the room temperature, the product was centrifuged by ethanol and deionized water for three times respectively and dried at 60 °C for 12 h.
X-ray diffraction (XRD) was obtained on BrukerD8 advance at a scanning speed of 10°/min in the 2θ range from 10 to 70 with Cu Kα radiation. Photoluminescence spectroscopy (PL) was recorded on a fluorescence spectrometer (FLS920, Edinburgh Instruments) upon continuous wave excitation of 980-nm laser diode. Scanning electron microscope (SEM) and energy dispersive spectrometer (EDS) were recorded on S-3400N-II.
Results and Discussion
Figure 1i presents the XRD patterns of the BaYF5:20%Yb3+, 2%Er3+ synthesized by different conditions. The diffraction peaks of all the samples can be readily indexed to the standard tetragonal-phase BaYF5 (JCPDS no.46-0039) except for Fig. 1i (a) owing to the generation of extra phase BaF2 at the pH value of 4. When the pH increased from 4 to 9, the crystalline of the sample was enhanced. In the meanwhile, the BaF2 phase disappeared as well. There was no extra peaks of other phase appeared, revealing that the varying experimental conditions have little influence on the crystal structure of the sample. It is noteworthy that all the diffraction peaks are shifted to higher 2θ side, which indicates the lattice constant becomes smaller because the radii of Er3+ or Yb3+ are smaller than those of Y3+ [25, 26]. Furthermore, it is easy to find the rules that when the reaction time increases, the intensity of the diffraction peaks is simultaneously enhanced. Similar conclusions are drawn when temperatures rise. It concludes that the above reaction conditions can promote the growth of BaYF5 crystals. EDS spectrum analysis of a specific sample was indicated in Fig. 1ii. As shown on the diagram, the presence of the elements of Ba, Y, F, Yb, and Er in the given sample was confirmed. According to the XRD and EDS results, Er3+ and Yb3+ were successfully doped into BaYF5. Figure 1v shows the SEM images of BaYF5 synthesized under different conditions. The as-prepared samples shown in Fig. 1v (A) are microspheres with a size of approximately 45 nm. However, they are not finely dispersed and aggregated to some extent. According to its XRD diagram in Fig. 1i (c), the size of the crystal can be roughly calculated by Scherrer’s equation:
where K is Scherrer constant (K equals 0.89), γ is the X-ray wavelength (γ equals 0.15405 nm), B is the full width at half maximum of diffraction peaks of samples, and θ is the diffraction angle of the observed peak [27, 28]. The strongest intensity of diffraction peak at 2θ = 26.689° was used to calculate the average size of crystal. The average size of crystal is estimated to be 41.7 nm which is closed to the size (45 nm) by observation of the SEM chart. As represented in Fig. 1v (B), when the reaction temperature was increased to 220 °C, the dispersions of the particles became relatively high. However, the size of the crystal was uneven and some larger particles with size of approximately 180 nm appeared. When the reaction time was prolonged to 24 h, the nanocrystals are relatively well dispersed with uniform particle morphology. The sizes are about 30 nm which are basically consistent with the estimates (24.9 nm) from the XRD data. Figure 1iii, iv shows the UC luminescence spectra of BaYF5:Er3+/Yb3+ synthesized via different experimental conditions under excitation at 980 nm. The main emission band of Er3+ is 520, 540, and 654 nm as a result of 2H11/2 → 4I15/2 (green), 4S3/2 → 4I15/2 (green), and 4F9/2 → 4I15/2 (red) transitions, respectively. In Fig. 1iii, iv, as the temperature increases, it is beneficial to the crystal growth of the product, while prolonging the reaction time, increasing pH has the same effect. The UC luminescence intensity can be enhanced due to the formation of higher crystalline. When the reaction time was prolonged, or pH was adjusted from 4 to 9, the nanoparticles have better crystalline owing to their higher dispersions and more uniform sizes.
Figure 2i demonstrates the XRD patterns of the BaYF5: xYb, 2%Er (x = 10%, 30%). All the diffraction peaks are perfectly matched with the standard pattern of BaYF5 crystals (JCPDS no.46-0039). It shows that the doping of rare earth ions does not affect the crystal growth. As shown in Fig. 2ii, when the Yb3+ concentration increases from 10 to 20%, the UC luminescence intensity rapidly rises until the Yb3+ concentration exceeds 20% on account of the concentration quenching. It is concluded that the 20% concentration is the optimum concentration.
Figure 3i exhibits the XRD patterns of the BaYF5:Yb3+/Er3+ nanocrystals obtained by adding different surfactants. All the diffraction peaks are perfectly matched with the standard card tetragonal-phase BaYF5 (JCPDS no.46-0039). When 5% polyetherimide (PEI) was added, the intensity of the diffraction peaks is enhanced, which indicates that PEI can promote the growth of BaYF5 crystals. Moreover, after the addition of citric acid, the diffraction peaks are shifted to lower angle. This proves that when citrate (CIT) was added, the cell volume of the sample becomes larger gradually. The other reason may be that citric acid is covered on the crystal surface, rare earth ions are hard to dope into the host lattices. Besides, the diffraction peaks become different from the others with a little flaw as the CIT/Y = 4:1. The conceivable reason lies in the high CIT concentration leading to the BaYF5 unit cell parameter change and lattice distortion. As illustrated in Fig. 3iii (A), when 5% PEI was added in ethanol, nanocrystals became massive clumps which consist of a large number of spherical particles with narrow size distribution. Figure 3iii (B) and (C) shows that when the surfactant with a concentration of CIT/Y = 1:1 was added, the overall size of crystal relatively became larger. As can be seen from the diagram, the sample tends to aggregate without obvious boundaries in some areas. As the surfactant concentration ratio rises to 4:1, the maximum size of the particles increases to 4 um with the surface covered by some other smaller spherical particles. As the surfactant concentration increases, the CIT coverage capacity is enhanced , leading to the formation of crystal clusters. As shown in Fig. 3ii, both green emission and red emission are enhanced after adding 5% PEI in ethanol. The long-chain amino groups of PEI can form the complex structures with metal ions by coordination. PEI can inhibit particle growth by tightly wrapping on the surface to improve the crystalline. On the contrary, after adding citric acid, the UC luminescence emission decreased greatly owing to the enlargement of crystal size and the decline of rare earth ion content.
Figure 4i shows the XRD pattern of products obtained from different fluoride sources. There are no peaks of impurities appear, demonstrating that the change of fluoride sources does not affect the crystallization of BaYF5. It is worth noting that there are fewer shifts of the diffraction peaks of samples obtained from NH4F or NaF than those of samples obtained from NaBF4. This indicates that NH4F and NaF released F− disorderly and rapidly, resulting in the difficulty of the control synthesis of crystals . As a consequence, the rare earth ions become difficult to enter into the host lattices. Figure 4iii represents the SEM images of the sample using NH4F and NaF as fluoride sources. The particles are similar to those nanocrystals synthesized by adding 5% PEI. However, the shapes are more irregular relative to those obtained from NaBF4. As can be seen from Fig. 4ii, the sample which used NaBF4 as fluoride source shows the highest UC emission efficiency owing to the benefits of the crystal growth generating a uniform sphere shape. Particles in smaller sizes will have more Er3+ on the submicron surface, causing more surface vibrations for conducting acceleration in red and green emission. Moreover, the distance among Er3+ becomes smaller and cross relaxation happens (2H11/2 + 4I15/2 → 4I9/2 + 4I13/2). As a result, the green band (2H11/2, 4S3/2 → 4I15/2) becomes easy to quench in smaller sizes, but the red band (4F9/2-4I15/2) becomes more difficult to quench [24, 31].
Figure 5 demonstrates the schematic energy levels of Yb3+ and Er3+. In the meanwhile, it depicts the UC luminescence process mechanisms explaining the generation of green and red emissions under 980-nm laser excitation. In the Yb3+/Er3+-codoped BaYF5 system, via absorbing the first 980-nm photon, Yb3+ ion in the 2F7/2 ground state transfers to the excited state 2F5/2. When it goes back to the ground state, the energy is transferred to Er3+ ion to populate the 4I11/2 state. The second 980-nm photon, or energy transfer from another excited Yb3+, can then pump Er3+ ion into 4F7/2 level. The lower energy states 2H11/2 and 4S3/2 can be populated by nonradiatively decaying 4F7/2 state. The transmissions of the electron from 2H11/2 and 4S3/2 to the 4I15/2 ground state emits green emissions. Alternatively, Er3+ ion in the 4I11/2 state may also nonradiatively relax to 4I13/2 state. 4F9/2 state of Er3+ can be populated by absorption of photon or energy transfer from Yb3+. The UC red emissions occur through the transition of 4F9/2 to 4I15/2. Some electrons in the 4F9/2 level may be excited to 2H9/2 via a phonon-assisted energy transfer process, and blue emissions can be observed. The emission bands at 520, 540, and 654 nm could be corresponding to electron transfer from the excited level 2H11/2, 4S3/2, and 4F9/2 to the ground state 4I15/2 of Er3+, respectively [19, 32, 33].
In summary, BaYF5:20%Yb3+, 2%Er3+ have been successfully synthesized via a convenient solvothermal method. It is found that the use of NaBF4 as a fluoride source or adding 5% PEI as surfactant can effectively improve the crystalline and particle dispersion which can promote the UC emission. Compared with PEI, as CIT concentration raised, the nanoparticles gradually become larger, which is inversely proportional to luminous properties. It is obvious that nanocrystals via 220 °C of heat treatment temperature for 24 h are an optimum reaction condition of the excellent luminescence properties. These behaviors might be attributed to their great uniform sizes, well dispersing, and high crystalline.
Dong B, Liu DP, Wang XJ, Yang T, Miao SM, Li CR (2007) Optical thermometry through infrared excited green upconversion emissions in Er3+-Yb3+ codoped Al2O3. Appl Phys Lett 90:181117
Wang M, Mi CC, Wang WX, Liu CH, Wu YF, Xu ZR et al (2009) Immunolabeling and NIR-excited fluorescent imaging of HeLa cells by using NaYF4: Yb, Er upconversion nanoparticles. ACS Nano 3:1580–1586
Maciel GS, Biswas A, Kapoor R, Prasad PN (2000) Blue cooperative upconversion in Yb3+-doped multicomponent sol-gel-processed silica glass for three-dimensional display. Appl Phys Lett 76:1978–1980
Dong H, Sun LD, Wang YF, Ke J, Si R, Xiao JW et al (2015) Efficient tailoring of upconversion selectivity by engineering local structure of lanthanides in NaxREF3+x nanocrystals. J Am Chem Soc 137:6569–6576
Xu DK, Li AM, Yao L, Lin H, Yang SH, Zhang YL (2017) Lanthanide-doped KLu2F7 nanoparticles with high upconversion luminescence performance: a comparative study by Judd-Ofelt analysis and energy transfer mechanistic investigation. Sci Rep 7:43189
Xu JT, He F, Cheng ZY, Lv RC, Dai YL, Gulzar A et al (2017) Yolk-structured upconversion nanoparticles with biodegradable silica shell for FRET sensing of drug release and imaging-guided chemotherapy. Chem Mater 29:7615–7628
Xu JT, Gulzar A, Liu YH, Bi HT, Gai SL, Liu B et al (2017) Integration of IR-808 sensitized upconversion nanostructure and MoS2 nanosheet for 808 nm NIR light triggered phototherapy and bioimaging. Small 13:1–13
Zou R, Huang JJ, Shi JP, Huang L, Zhang XJ, Wong KL et al (2017) Silica shell-assisted synthetic route for mono-disperse persistent nanophosphors with enhanced in vivo recharged near-infrared persistent luminescence. Nano Res 10:2070–2082
Xu JT, Kuang Y, Lv RC, Yang PP, Li CX, Bi HT et al (2017) Charge convertibility and near infrared photon co-enhanced cisplatin chemotherapy based on upconversion nanoplatform. Biomaterials 130:42–55
Xu JT, Yang PP, Sun MD, Bi HT, Liu B, Yang D et al (2017) Highly emissive dye-sensitized upconversion nanostructure for dual-photosensitizer photodynamic therapy and bioimaging. ACS Nano 11:4133–4144
Zou R, Gong SM, Shi JP, Jiao J, Wong KL, Zhang HW et al (2017) Magnetic-NIR persistent luminescent dual-modal ZGOCS@ MSNs@ Gd2O3 core-shell nanoprobes for in vivo imaging. Chem Mater 29:3938–3946
Wei W, Zhang Y, Chen R, Goggi JL, Ren N, Huang L et al (2014) Cross relaxation induced pure red upconversion in activator-and sensitizer-rich lanthanide nanoparticles. Chem Mater 26:5183–5186
Sun RJ, Qiu PY, Yin T, Gao G, Fu HL, Wang K et al (2016) Potassium sodium tartrate-assisted hydrothermal synthesis of BaLuF5: Yb3+/Er3+ nanocrystals. Particuology 24:164–169
del-Castillo J, Yanes AC, Abé S, Smet PF. Site selective spectroscopy in BaYF5: RE3+ (RE = Eu, Sm) nano-glass-ceramics. Journal of Alloys and Compounds. 2015;635:136-141
Zhang WH, Ouyang SY, Zhang ZX, Zhang YP, Xia HP (2015) Luminescent properties of Eu3+-doped glass ceramics containing BaGdF5 nanocrystals under NUV-excitation for W-LEDs. Ceram Int 41:14035–14040
Liu F, Wang YS, Chen DQ, Yu YL, Ma E, Zhou LH et al (2007) Upconversion emission of a novel glass ceramic containing Er3+: BaYF5 nano-crystals. Mater Lett 61:5022–5025
Hwang BC, Jiang S, Luo T, Watson J, Sorbello G, Peyghambarian N (2000) Cooperative upconversion and energy transfer of new high Er 3+- and Yb 3+–Er 3+-doped phosphate glasses. J Opt Soc Am B 17:833–839
Yang DM, Li CX, Li GG, Shang MM, Kang XK, Lin J (2011) Colloidal synthesis and remarkable enhancement of the upconversion luminescence of BaGdF5: Yb3+/Er3+ nanoparticles by active-shell modification. J Mater Chem 21:5923–5927
Grzyb T, Balabhadra S, Przybylska D, Węcławiak M (2015) Upconversion luminescence in BaYF5, BaGdF5, and BaLuF5, nanocrystals doped with Yb3+/Ho3+, Yb3+/Er3+, or Yb3+/Tm3+, ions. J Alloys Compounds 649:606–616
Chen XP, Zhang QY, Yang CH, Chen DD, Zhao C (2009) Comparative investigation on structure and luminescence properties of fluoride phosphors codoped with Er3+/Yb3+. Spectrochim Acta A Mol Biomol Spectrosc 74:441–445
Jung HJ, Ahn KY, Choi SC, Lee SH, Aldinger F (2008) Low pressure sintering of sialon using different sintering additives. J Ceram Soc Jpn 116:130–136
Zeng JH, Su J, Li ZH, Yan RX, Li YD (2005) Synthesis and upconversion luminescence of hexagonal-phase NaYF4:Yb, Er3+ phosphors of controlled size and morphology. Adv Mater 17:2119–2123
Sun YJ, Chen Y, Tian LJ, Yu Y, Kong XG, Zhang JW et al (2007) Controlled synthesis and morphology dependent upconversion luminescence of NaYF4: Yb. Er nanocrystals Nanotechnology 18:275609
Sun JY, Xian JB, Du HY (2011) Hydrothermal synthesis of BaYF5: Yb3+/Er3+ upconversion luminescence submicrospheres by a surfactant-free aqueous solution route. J Phys Chem Solids 72:207–213
Du HY, Zhang WH, Sun JY (2011) Structure and upconversion luminescence properties of BaYF5: Yb3+, Er3+ nanoparticles prepared by different methods. J Alloys Compd 509:3413–3418
Cao ZM, Zhou SS, Jiang GC, Chen YH, Duan CK, Yin M (2014) Temperature dependent luminescence of Dy3+ doped BaYF5 nanoparticles for optical thermometry. Curr Appl Phys 14:1067–1071
Monshi A, Foroughi MR, Monshi MR (2012) Modified Scherrer equation to estimate more accurately nano-crystallite size using XRD. World J Nano Sci Eng 2:154–160
Burton AW, Ong K, Rea T, Chan IY (2009) On the estimation of average crystallite size of zeolites from the Scherrer equation: a critical evaluation of its application to zeolites with one-dimensional pore systems. Microporous Mesoporous Mater 117:75–90
Zhang CM, Ma PA, Li CX, Li GG, Huang SS, Yang DM et al (2011) Controllable and white upconversion luminescence in BaYF5: Ln3+ (Ln = Yb, Er, Tm) nanocrystals. J Mater Chem 21:717–723
Li CX, Yang J, Quan ZW, Yang PP, Kong DY, Lin J (2007) Different microstructures of β-NaYF4 fabricated by hydrothermal process: effects of pH values and fluoride sources. Chem Mater 19:4933–4942
Shan JN, Uddi M, Wei R, Yao N, Ju YG (2010) The hidden effects of particle shape and criteria for evaluating the upconversion luminescence of the lanthanide doped nanophosphors. J Phys Chem C 114:2452–2461
Niu N, Yang PP, Liu YC, Li CX, Wang D, Gai SL et al (2011) Controllable synthesis and up-conversion properties of tetragonal BaYF5: Yb/Ln (Ln= Er, Tm, and Ho) nanocrystals. J Colloid Interface Sci 362:389–396
Tian G, Gu ZJ, Zhou LJ, Yin WY, Liu XX, Yan L et al (2012) Mn2+ dopant-controlled synthesis of NaYF4: Yb/Er upconversion nanoparticles for in vivo imaging and drug delivery. Adv Mater 24:1226–1231
This work was supported by the National Natural Science Foundation of China (51002034) and the Natural Science Foundation of Guangdong Province (2014A030313466).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Yao, J., Zhao, F., Pan, C. et al. Controlled Synthesis of BaYF5:Er3+, Yb3+ with Different Morphology for the Enhancement of Upconversion Luminescence. Nanoscale Res Lett 12, 633 (2017) doi:10.1186/s11671-017-2390-4
- Er3+/Yb3+ codoped
- Luminescent properties